State-of-the-Art of Polymer/Fullerene C60 Nanocomposite Membranes for Water Treatment: Conceptions, Structural Diversity and Topographies

To secure existing water resources is one of the imposing challenges to attain sustainability and ecofriendly world. Subsequently, several advanced technologies have been developed for water treatment. The most successful methodology considered so far is the development of water filtration membranes for desalination, ion permeation, and microbes handling. Various types of membranes have been industrialized including nanofiltration, microfiltration, reverse osmosis, and ultrafiltration membranes. Among polymeric nanocomposites, nanocarbon (fullerene, graphene, and carbon nanotubes)-reinforced nanomaterials have gained research attention owing to notable properties/applications. Here, fullerene has gained important stance amid carbonaceous nanofillers due to zero dimensionality, high surface areas, and exceptional physical properties such as optical, electrical, thermal, mechanical, and other characteristics. Accordingly, a very important application of polymer/fullerene C60 nanocomposites has been observed in the membrane sector. This review is basically focused on talented applications of polymer/fullerene nanocomposite membranes in water treatment. The polymer/fullerene nanostructures bring about numerous revolutions in the field of high-performance membranes because of better permeation, water flux, selectivity, and separation performance. The purpose of this pioneering review is to highlight and summarize current advances in the field of water purification/treatment using polymer and fullerene-based nanocomposite membranes. Particular emphasis is placed on the development of fullerene embedded into a variety of polymer membranes (Nafion, polysulfone, polyamide, polystyrene, etc.) and effects on the enhanced properties and performance of the resulting water treatment membranes. Polymer/fullerene nanocomposite membranes have been developed using solution casting, phase inversion, electrospinning, solid phase synthesis, and other facile methods. The structural diversity of polymer/fullerene nanocomposites facilitates membrane separation processes, especially for valuable or toxic metal ions, salts, and microorganisms. Current challenges and opportunities for future research have also been discussed. Future research on these innovative membrane materials may overwhelm design and performance-related challenging factors.


Introduction
Clean water is vivacious for human beings and the ecological world environment [1,2]. To achieve unsoiled water, implementation of water treatment or purification technologies phase inversion, electrospinning, and solid phase synthesis routes. The ensuing novel membrane materials may have capabilities to overwhelm the challenging aqueous environment for the filtration of undesirable contaminants. In other words, this article offers a groundbreaking and original review on polymer and fullerene-based membrane materials. Despite remarkable properties and the vast potential, devoted future research efforts are desirable to form high-performance nanocomposite membranes for water purification applications and to overcome the associated challenges. Future developments in the field of novel functional polymer/fullerene C 60 nanocomposite membranes are not possible for researchers before getting prior knowledge of the reported literature in this field.

Fullerene
Fullerene is a symmetrical zero-dimensional nano-allotrope of carbon [23]. It is a hollow ball-like nanostructure having sp 2 hybridized carbon atoms in its architecture [24]. The carbon atoms in fullerene form a π conjugation system [25,26]. It is made up of unique polygons, i.e., pentagons and hexagons. The cage-like fullerene nanostructure is~1 nm [27]. Fullerene was primarily discovered in 1985 [28]. Depending upon the number of carbon atoms in the structure, the fullerene molecules can be of several types such as C 24 , C 28 , C 60 , C 70 , and C 120 ( Figure 1) [29]. Fullerene C 60 is a commonly known fullerene molecule also referred to as buckminsterfullerene. Then, the next widely researched form of fullerene is C 70 . Fullerene molecules have revealed sole optical, electrical, magnetic, thermal, mechanical, and biomedical possessions [30][31][32]. Fullerene molecules have been primed using numerous procedures such as the microwave synthesis, arc discharge, plasma techniques, chemical vapor deposition, and numerous chemical approaches [31][32][33]. Nanocarbons such as graphene, carbon nanotube, and nanodiamond have been applied in essential technical applications including nanocomposite formation [34][35][36][37]. Nanocomposites have been formed using the in situ method, solution mixing, melt processing, spinning, printing, and other practices [38][39][40]. Fullerene molecules own exceptional physical features for nanocomposite applications [41][42][43][44]. With polymers, fullerene molecules may form an electron donor-acceptor relationship [45]. The solubility properties of fullerene in number of solvents have been explored for the nanocomposite formation [46][47][48]. The polymers such as poly(vinylpyrrolidone) have also been employed to solubilize fullerene molecules [49][50][51]. Applications areas of fullerene, functional fullerene, and nanocomposites have been observed in optoelectronics [52][53][54], solar cells [55], sensors [56], drug delivery [57], and other practical fields. In the membrane application, fullerene has been reinforced in polymeric matrices to influence final properties [58]. As compared to other nanocarbons, fullerene has a higher surface area to interact with polymers and own a lower aggregation tendency and better dispersion properties [59]. For water treatment purposes, fullerene addition may enhance homogeneity in polymeric membranes; however, appropriate surfactants and stabilizing agents need to be included to form high-performance materials [60,61]. Mostly, fullerene C 60 molecules are reinforced in polymeric matrices to form water filtration membranes. Other fullerene forms have been rarely studied in polymeric membranes.

Polymer/Fullerene Nanocomposite
Polymer/fullerene nanocomposites have been considered for superior optical, electrical, thermal, mechanical, and processability features [131][132][133]. However, during the polymer/fullerene nanocomposite formation, agglomeration can cause major hinderance to the production of high-performance nanomaterials. The aggregation of fullerene molecules may cause poor solubility in organic solvents [134]. Consequently, the large-scale processing of polymer/fullerene nanocomposites has been studied [135]. To resolve this issue, functional fullerene molecules have been reinforced in polymeric matrices [136,137]. A range of thermoplastics, thermosets, and conjugated polymers have been used to form nanocomposites with fullerene [138,139]. Polymer/fullerene nanocomposites have been applied in wide-ranging methodological fields such as electronics [140], supercapacitors [141], and solar cells [142]. Fullerene C60 has been physically or covalently linked with host polymers to enhance final nanomaterial characteristics [143,144]. The systematic studies on the polymer/fullerene nanocomposites have escorted towards polymeric membranes [145]. In this regard, numerous filtration membranes have been developed using varying polymers (polyamide, polystyrene, polysulfone, etc.) and the fullerene C60 nanofiller [146][147][148]. Nanocomposite membranes have been focused on due to its chemical stability, mechanical resilience, rigidity, porosity, and inexpensiveness [149][150][151]. The inclusion of fullerene contents have significantly improved technological membrane parameters towards the remediation of environmental effluents [152]. Kitjanon et al. [153] developed and studied the cis-1,4-polyisoprene and C60-based nanocomposite membranes via coarse-grained molecular dynamics simulation. Nanoparticles with 0-32 phr fullerene were loaded, and then, simulations were performed over 200 microseconds. The photographs of the cis-1,4polyisoprene and C60-based nanocomposite are given in Figure 3. In addition, the experimental results for the glass transition temperature, mechanical, and thermodynamical properties were investigated for the high-performance nanocomposites.  [130]. Reproduced with permission from Elsevier.

Polymer/Fullerene Nanocomposite
Polymer/fullerene nanocomposites have been considered for superior optical, electrical, thermal, mechanical, and processability features [131][132][133]. However, during the polymer/fullerene nanocomposite formation, agglomeration can cause major hinderance to the production of high-performance nanomaterials. The aggregation of fullerene molecules may cause poor solubility in organic solvents [134]. Consequently, the large-scale processing of polymer/fullerene nanocomposites has been studied [135]. To resolve this issue, functional fullerene molecules have been reinforced in polymeric matrices [136,137]. A range of thermoplastics, thermosets, and conjugated polymers have been used to form nanocomposites with fullerene [138,139]. Polymer/fullerene nanocomposites have been applied in wide-ranging methodological fields such as electronics [140], supercapacitors [141], and solar cells [142]. Fullerene C 60 has been physically or covalently linked with host polymers to enhance final nanomaterial characteristics [143,144]. The systematic studies on the polymer/fullerene nanocomposites have escorted towards polymeric membranes [145]. In this regard, numerous filtration membranes have been developed using varying polymers (polyamide, polystyrene, polysulfone, etc.) and the fullerene C 60 nanofiller [146][147][148]. Nanocomposite membranes have been focused on due to its chemical stability, mechanical resilience, rigidity, porosity, and inexpensiveness [149][150][151]. The inclusion of fullerene contents have significantly improved technological membrane parameters towards the remediation of environmental effluents [152]. Kitjanon et al. [153] developed and studied the cis-1,4-polyisoprene and C 60 -based nanocomposite membranes via coarse-grained molecular dynamics simulation. Nanoparticles with 0-32 phr fullerene were loaded, and then, simulations were performed over 200 microseconds. The photographs of the cis-1,4-polyisoprene and C 60 -based nanocomposite are given in Figure 3. In addition, the experimental results for the glass transition temperature, mechanical, and thermodynamical properties were investigated for the high-performance nanocomposites. Membranes 2023, 13, 27 6 of 22

Implication of Polymer/Fullerene Nanocomposite Membranes in Water Treatment
Polymer/fullerene nanocomposite membranes have been investigated for effective salt removal from water, toxic ion separation, ion pair separation, recovery of expensive metals, and pathogenic microorganisms separation or deterioration [154]. In the sorption method, a huge range of metal ions can be recovered such as nickel, zinc, copper, cobalt, mercury, lead, arsenic, and cadmium [155][156][157]. The design of polymer/fullerene nanocomposite membranes and surface defects may influence their sorption capacities towards metals [158]. Moreover, nanocomposite membranes show better retention time [159]. Perera et al. [160] formed thin-film reverse osmosis membranes having functional hydroxy fullerene C60. The membranes revealed a high water flux of 26.1 L/(m 2 •h) and the optimum salt rejection. Moreover, the hydroxy functional fullerene C60-derived membranes presented a high separation efficiency towards Mg 2+/ Li + (separation factor: 13.1). The nanocomposite membranes were found effective for the recovery of Li + ions from seawater [161]. Liu et al. [162] reported epoxy-based membranes with fullerene C60-grafted graphene oxide. Water desalination and ion permeation were studied through the membranes. Figure 4 displays the fabrication procedure, water desalination system, and representation of anions/cations blockage on the membrane surface. The membranes had a high water flux of up to 10.85 L/(m 2 •h•bar) and 0.1883 mol/(m 2 •h•bar) for water desalination and ion permeation, respectively. The inclusion of fullerene C60 revealed fine water adsorption for large water quantities. Table 1 displays the filtration performances of a few systems showing polymeric membranes with fullerene nanoparticles.

Implication of Polymer/Fullerene Nanocomposite Membranes in Water Treatment
Polymer/fullerene nanocomposite membranes have been investigated for effective salt removal from water, toxic ion separation, ion pair separation, recovery of expensive metals, and pathogenic microorganisms separation or deterioration [154]. In the sorption method, a huge range of metal ions can be recovered such as nickel, zinc, copper, cobalt, mercury, lead, arsenic, and cadmium [155][156][157]. The design of polymer/fullerene nanocomposite membranes and surface defects may influence their sorption capacities towards metals [158]. Moreover, nanocomposite membranes show better retention time [159]. Perera et al. [160] formed thin-film reverse osmosis membranes having functional hydroxy fullerene C 60 . The membranes revealed a high water flux of 26.1 L/(m 2 ·h) and the optimum salt rejection. Moreover, the hydroxy functional fullerene C 60 -derived membranes presented a high separation efficiency towards Mg 2+ /Li + (separation factor: 13.1). The nanocomposite membranes were found effective for the recovery of Li + ions from seawater [161]. Liu et al. [162] reported epoxy-based membranes with fullerene C 60 -grafted graphene oxide. Water desalination and ion permeation were studied through the membranes. Figure 4 displays the fabrication procedure, water desalination system, and representation of anions/cations blockage on the membrane surface. The membranes had a high water flux of up to 10.85 L/(m 2 ·h·bar) and 0.1883 mol/(m 2 ·h·bar) for water desalination and ion permeation, respectively. The inclusion of fullerene C 60 revealed fine water adsorption for large water quantities. Table 1 [162]. Reproduced with permission from American Chemical Society.  60 14-59 33-34 nm to 53-55 nm - [167] The biocompatibility of fullerene is an ultimate requirement to ensure the safety of drinking water [168]. Fullerene nanofillers embedded into various polymeric membranes influence the resulting membranes performance. The size, shape, and surface properties of fullerenes have been found important to enhance the solute selectivity, water permeability, and stability of nanocomposite membranes. Fullerene nanofillers have been used (e) graphene oxide-C 60 membrane inside a water desalination setup; (f,g) schematic setup of a flat membrane made of graphene oxide and a C 60 hybrid for water desalination [162]. Reproduced with permission from American Chemical Society. The biocompatibility of fullerene is an ultimate requirement to ensure the safety of drinking water [168]. Fullerene nanofillers embedded into various polymeric membranes influence the resulting membranes performance. The size, shape, and surface properties of fullerenes have been found important to enhance the solute selectivity, water permeability, and stability of nanocomposite membranes. Fullerene nanofillers have been used to achieve desirable pore sizes, larger surface areas, and unique surface functionalities, improving the overall membrane performance. For the fabrication of polymer/fullerene nanocomposite membranes, the surface chemistry of fullerene has been considered important to accomplish better membrane stability [169]. The presence of physical or covalent bonding of fullerene with polymers in nanocomposite membranes have been found to improve hydrophilicity and anti-bacterial, anti-fouling, and water flux performance. Moreover, interactions between fullerene and polymers also aid in the improved membrane thermomechanical stability and long-term durability during filtration and hydraulic cleaning processes. In addition, polymer/fullerene membranes possess low toxicity, long-term organic solvent stability, and enhanced membrane operating times even at higher temperatures. Molecular dynamics (MD) simulations were used to gain insights on the interactions of polymer with fullerene in membranes [170]. The interactions between a single fullerene C 60 molecule and a membrane were evaluated by computing the free energy as a function of the distance between the C 60 molecule and the polymer layer. The fullerene molecule was found to be absorbed into the polymer hydrophobic part with a marked increase in the stability of the membrane (~30 kcal/mol) and cause no disruption of the hydrophobic environment. According to MD studies, initial fullerene clusters need to be disaggregated to release from the membranes. Furthermore, to make the fullerene molecule soluble from the polymeric membranes, both the energetic and kinetic barriers need to be overcome. Thus, the studies revealed the kinetic stability of polymer/fullerene nanocomposite membranes, and these membranes were not found easily degradable in aqueous environments.

Nafion/Fullerene Nanocomposite Membranes for Water Treatment
Nafion is a sulfonated tetrafluoroethylene-based fluoropolymer-copolymer [171,172]. It is a widely used synthetic polymer. It has ionic properties such as ionomers. Nafion has been commonly used to form commercial membranes for energy, electronics, and environmental applications [173,174]. Nafion and fullerene-based nanocomposite membranes have been devised [175]. The use of hydroxy-modified fullerene in Nafion results in fine photoconductivity and antimicrobial characteristics. Tasaki et al. [176] fabricated a Nafion/fullerene C 60 nanocomposite with the solution casting technique. The neat fullerene C 60 and the polyhydroxy fullerene were used as nanofillers. Figure 5 demonstrates the optical micrographs of the solution-cast nanocomposite membranes. Two types of membranes were prepared, i.e., through the doping process and by solution casting. In the doping process, toluene was used as a solvent. On the other hand, dimethyl acetamide was used as a solvent in the solution route. In the doping route, functional fullerene nanoparticles formed large aggregates. In the case of the solution route, finely dispersed fullerene and functional fullerene nanoparticles can be observed. Thus, the solution route was found ideal due to better miscibility properties between the Nafion matrix and the nanofiller. Figure 6 expresses the molecular dynamic simulations of the Nafion/fullerene nanocomposite membranes. The fullerene molecule can be seen totally wrapped by the Nafion oligomer, screening better mutual interactions. The water uptake of the membranes was measured through soaking in water (wet condition) and under a 25% RH (dry condition). The 1 wt % Nafion/C 60 and 3 wt % Nafion/C 60 membranes were tested. Both the Nafion/C 60 nanocomposite membranes were found to hold more water than the neat Nafion, under a 25% RH. Consequently, the higher wet and dry water uptakes of nanocomposite membranes were observed, compared with those of the neat Nafion membrane. The water molecules were suggested to be trapped in the interfaces between the C 60 aggregates and Nafion domains, depending upon the morphological form of the nafion/C 60 nanocomposite. In the Nafion/fullerene nanofiltration membranes, the internal porosity and permeability were found to be affected by the packing of the polymer chains and dispersion of the fullerene nanoparticles [175]. The presence of fullerene was supposed to interrupt the packing manner of the polymer chains and interfacial morphology to generate nanopores in the Nafion/fullerene nanofiltration membranes for ion separation purposes. Nevertheless, few Nafion/fullerene systems have been studied up till now for water treatment, so further research efforts are found desirable in this category. was supposed to interrupt the packing manner of the polymer chains and interfacial morphology to generate nanopores in the Nafion/fullerene nanofiltration membranes for ion separation purposes. Nevertheless, few Nafion/fullerene systems have been studied up till now for water treatment, so further research efforts are found desirable in this category. Figure 5. Optical micrographs of Nafion/C60 fullerene nanocomposites (a) and Nafion/polyhydroxy fullerene nanocomposites (b) by doping and Nafion/C60 fullerene nanocomposites (c) and Nafion/polyhydroxy fullerene nanocomposites (d) by solution casting [176]. Reproduced with permission from Elsevier. Figure 6. (a) Initial structure of C60 and Nafion oligomers; (b) snapshots of Nafion oligomers; (c) C60 and Nafion oligomers; and (d) polyhydroxy and Nafion oligomers (taken after 1 ns molecular dynamic simulations) [176]. Reproduced with permission from Elsevier.

Polysulfone/Fullerene Nanocomposite Membranes in Water Treatment
Polysulfone is a commercial thermoplastic polymer [177]. Polysulfone own fine properties of chemical, thermal, and mechanical stability. Owing to unique processability and Figure 5. Optical micrographs of Nafion/C 60 fullerene nanocomposites (a) and Nafion/polyhydroxy fullerene nanocomposites (b) by doping and Nafion/C 60 fullerene nanocomposites (c) and Nafion/polyhydroxy fullerene nanocomposites (d) by solution casting [176]. Reproduced with permission from Elsevier. was supposed to interrupt the packing manner of the polymer chains and interfacial morphology to generate nanopores in the Nafion/fullerene nanofiltration membranes for ion separation purposes. Nevertheless, few Nafion/fullerene systems have been studied up till now for water treatment, so further research efforts are found desirable in this category. Figure 5. Optical micrographs of Nafion/C60 fullerene nanocomposites (a) and Nafion/polyhydroxy fullerene nanocomposites (b) by doping and Nafion/C60 fullerene nanocomposites (c) and Nafion/polyhydroxy fullerene nanocomposites (d) by solution casting [176]. Reproduced with permission from Elsevier. and Nafion oligomers; and (d) polyhydroxy and Nafion oligomers (taken after 1 ns molecular dynamic simulations) [176]. Reproduced with permission from Elsevier.

Polysulfone/Fullerene Nanocomposite Membranes in Water Treatment
Polysulfone is a commercial thermoplastic polymer [177]. Polysulfone own fine properties of chemical, thermal, and mechanical stability. Owing to unique processability and (c) C 60 and Nafion oligomers; and (d) polyhydroxy and Nafion oligomers (taken after 1 ns molecular dynamic simulations) [176]. Reproduced with permission from Elsevier.

Polysulfone/Fullerene Nanocomposite Membranes in Water Treatment
Polysulfone is a commercial thermoplastic polymer [177]. Polysulfone own fine properties of chemical, thermal, and mechanical stability. Owing to unique processability and physical features, polysulfone has found wide-ranging applications in membranes, coating, nanocomposites, and other technical fields [178]. Penkova et al. [179] fabricated mixed-matrix membranes of polysulfone and fullerene C 60 (contents up to 5 wt %). The nanocomposite membrane with a 5 wt % fullerene content revealed fine transport properties towards the pervaporation of an ethyl acetate-water mixture. The sorption and contact angle measurement data for the membranes are given in Table 2. The inclusion of nanofillers enhanced the sorption characteristics. Moreover, the hydrophilic features of the membrane surface were improved with the fullerene addition. The pervaporation mechanism can be explained through the solution-diffusion process [180]. Especially, the permeability is directly related to the solubility and diffusivity of the solute molecules. In this way, the mass transfer of analyte and water through the membranes can be analyzed. However, limited polysulfone/fullerene systems have been studied so far, and thorough research efforts needed to form high-performance membranes in this category. Table 2. Sorption characteristics and contact angles of polysulfone and polysulfone/fullerene C 60 dense membranes [179]. Reproduced with permission from Springer.

Polyamide/Fullerene Nanocomposite Membranes towards Water Treatment
Polyamide is a thermoplastic polymer having repeating amide bonds in the backbone. Polyamides occur naturally and can be synthesized using diamine and dicarboxylic acid monomers [181]. Polyamide has been effectively used in membrane applications [182]. Plisko et al. [167] designed a polyamide and hydroxy functional fullerene C 60 -based thin-film nanocomposite membrane for water treatment. It has been observed that the inclusion of a 5 wt % nanofiller promoted antifouling features and organic matter elimination properties of the membranes. Dmitrenko et al. [166] adopted a polyamide, i.e., polyphenylene isophthalamide filled with 5 wt % fullerene derivatives (carboxyfullerene, polyhydroxylated fullerene and fullerene derivative with L-arginine). In this regard, various pervaporation membranes have been designed as polyphenylene isophthalamide/fullerene (PA/F), polyphenylene isophthalamide/carboxyfullerene (PA/CF), polyphenylene isophthalamide/fullerene derivative with L-arginine (PA/AF), and polyphenylene isophthalamide/polyhydroxylated fullerene (PA/HF). The solid phase synthesis route was used to fabricate mixed matrix pervaporation membranes (Figure 7). The transport properties were studied for the azeotropic methanoltoluene (72/28 wt %) mixture. Figure 8 depicts the permeation flux for the mixed matrix pervaporation, which was increased with the increasing methanol content in feed. Moreover, the inclusion of fullerene derivative to the polymeric membranes enhanced the permeation flux in order of PA < PA/F < PA/CF < PA/AF < PA/HF. Relative to the neat pervaporation membrane, the permeation flux of the nanocomposite membrane was increased by 1.6 times, due to the effect of the inclusion of fullerene nanoparticles. Furthermore, the nanocomposite membranes have enhanced the surface roughness and the surface hydrophilicity properties, relative to the neat polyphenylene isophthalamide membrane. The polyhydroxylated fullerene-based membrane revealed superior performance compared with the other nanocomposite membranes. Consequently, the PA/HF membrane with a 5 wt % nanofiller content increased the permeation flux to 0.084-0.214 kg/(m 2 ·h) and resulted in the selectivity of 95.9 wt % for methanol. The results were attributed to the affinity of the polyhydroxy functionality of the fullerene molecules permeating methanol. The results were also suggestive of the nanocomposite membrane pore size modification with the addition of altered fullerene derivatives [183]. Comprehensive efforts are still desirable to explore the interaction of the modified fullerene nanoparticles with the polyamide chains actually operating to promote the membrane permeation and selectivity. of 95.9 wt % for methanol. The results were attributed to the affinity of the polyhydroxy functionality of the fullerene molecules permeating methanol. The results were also suggestive of the nanocomposite membrane pore size modification with the addition of altered fullerene derivatives [183]. Comprehensive efforts are still desirable to explore the interaction of the modified fullerene nanoparticles with the polyamide chains actually operating to promote the membrane permeation and selectivity.   [166]. PA, polyphenylene isophthalamide; PA/F, polyphenylene isophthalamide/fullerene; PA/CF, polyphenylene isophthalamide/carboxyfullerene; PA/AF, polyphenylene isophthalamide/fullerene derivative with L-arginine; PA/HF, polyphenylene isophthalamide/polyhydroxylated fullerene. Reproduced with permission from Elsevier.

Polystyrene/Fullerene Nanocomposite Membranes for Water Treatment
Polystyrene is a widely used commercial thermoplastic polymer [184,185]. Polystyrene is usually made from styrene monomer. It is an inexpensive, light-weight, clear, hard, of 95.9 wt % for methanol. The results were attributed to the affinity of the polyhydroxy functionality of the fullerene molecules permeating methanol. The results were also suggestive of the nanocomposite membrane pore size modification with the addition of altered fullerene derivatives [183]. Comprehensive efforts are still desirable to explore the interaction of the modified fullerene nanoparticles with the polyamide chains actually operating to promote the membrane permeation and selectivity. Figure 7. Graphical development of novel polyphenylene isophthalamide pervaporation (PV) membranes modified with various types of fullerene C60 derivatives [166]. Reproduced with permission from Elsevier.

Polystyrene/Fullerene Nanocomposite Membranes for Water Treatment
Polystyrene is a widely used commercial thermoplastic polymer [184,185]. Polystyrene is usually made from styrene monomer. It is an inexpensive, light-weight, clear, hard, and brittle polymer. Polystyrene has been frequently used to form nanocomposites. Alekseeva et al. [163] formed fullerene C 60 -filled polystyrene nanocomposite. The ultrafiltration membranes were designed using the phase inversion technique. The static protein sorption tests were carried out for the polystyrene/C 60 nanocomposite membranes. With the fullerene nanoparticle loading, protein sorption was reduced along with the flux reduced recovery rates. The result was observed due to better fullerene dispersion and barrier effects in the membranes. Moreover, the Langmuir model was used to study the Cu 2+ ions removal efficiency. It was found that the fullerene addition enhanced the membrane affinity towards Cu 2+ ions due to better interactions. The fullerene C 60 has also been incorporated in polystyrene blend matrices to form water treatment membranes [186,187]. von Reitzenstein et al. [188] performed a comparative study on neat polystyrene, polystyrene/fullerene C 60 , polystyrene/graphene oxide, and polystyrene/multi-walled carbon nanotubes. The electrospinning technique was used to form nanocomposite nanofibers. Electrospun nanofibers were then used to form nanofiltration membranes. The inclusion of nanofillers in the electrospun polystyrene nanofibers slightly enhanced the diameter, reduced the bead formation and caused the homogeneous surface pore size distribution. Figure 9 displays the surface pore volume distribution of the nanofiber. The mean pore diameters of the neat polymer and polystyrene/graphene oxide was found similar, which were 70-90 nm. and brittle polymer. Polystyrene has been frequently used to form nanocomposites. Alekseeva et al. [163] formed fullerene C60-filled polystyrene nanocomposite. The ultrafiltration membranes were designed using the phase inversion technique. The static protein sorption tests were carried out for the polystyrene/C60 nanocomposite membranes. With the fullerene nanoparticle loading, protein sorption was reduced along with the flux reduced recovery rates. The result was observed due to better fullerene dispersion and barrier effects in the membranes. Moreover, the Langmuir model was used to study the Cu 2+ ions removal efficiency. It was found that the fullerene addition enhanced the membrane affinity towards Cu 2+ ions due to better interactions. The fullerene C60 has also been incorporated in polystyrene blend matrices to form water treatment membranes [186,187]. von Reitzenstein et al. [188] performed a comparative study on neat polystyrene, polystyrene/fullerene C60, polystyrene/graphene oxide, and polystyrene/multi-walled carbon nanotubes. The electrospinning technique was used to form nanocomposite nanofibers. Electrospun nanofibers were then used to form nanofiltration membranes. The inclusion of nanofillers in the electrospun polystyrene nanofibers slightly enhanced the diameter, reduced the bead formation and caused the homogeneous surface pore size distribution. Figure 9 displays the surface pore volume distribution of the nanofiber. The mean pore diameters of the neat polymer and polystyrene/graphene oxide was found similar, which were 70-90 nm. On the other hand, the polystyrene/fullerene C60 and the polystyrene/multi-walled carbon nanotube had a reduced mean pore diameter of 50-70 nm. The effect was observed probably due to more stability and less pore formation tendency of fullerene and nanotube-filled nanocomposites. The transmission electron microscopy (TEM) was used to inspect the morphologies of the neat polystyrene nanofiber and the nanocarbon-dispersed nanocomposite nanofiber ( Figure 10). The polystyrene/graphene oxide-based nanofiber showed a flaky appearance due to the presence of nanosheets. The nanotube can be observed as tangled threads in the polystyrene/multi-walled carbon nanotube nanocomposites. The polystyrene/fullerene nanofibers were opaque and dense, although few fullerene aggregates can be identified as flaky edges on the fiber surface. The polymer/nanocar- Figure 9. Distribution of the pore volume measured from scanning electron microscopy of nanofibers [188]. PS, polystyrene; C 60 -PS, fullerene-polystyrene; MWCNT-PS, multi-walled carbon nanotube-polystyrene; GO-PS, graphene oxide-polystyrene. Reproduced with permission from Elsevier.
On the other hand, the polystyrene/fullerene C 60 and the polystyrene/multi-walled carbon nanotube had a reduced mean pore diameter of 50-70 nm. The effect was observed probably due to more stability and less pore formation tendency of fullerene and nanotubefilled nanocomposites. The transmission electron microscopy (TEM) was used to inspect the morphologies of the neat polystyrene nanofiber and the nanocarbon-dispersed nanocomposite nanofiber ( Figure 10). The polystyrene/graphene oxide-based nanofiber showed a flaky appearance due to the presence of nanosheets. The nanotube can be observed as tangled threads in the polystyrene/multi-walled carbon nanotube nanocomposites. The polystyrene/fullerene nanofibers were opaque and dense, although few fullerene aggregates can be identified as flaky edges on the fiber surface. The polymer/nanocarbon nanofibers for the filtration membranes must be further investigated for the mechanism of pore creation, pore formation frequency control, and precise nanofiber dimensions [189]. bon nanofibers for the filtration membranes must be further investigated for the mechanism of pore creation, pore formation frequency control, and precise nanofiber dimensions [189].

Challenges, Future, and Summary
There is a mammoth necessity of better-quality approaches to the use of fullerenes and derived nanomaterials in high tech industries [190]. Most prominently, fullerene-derived nanomaterials have been absorbed for membranes or coatings [191], electronics [192], energy devices [193], biomedical areas [194], and other fields. The future implication of fullerene-based nanomaterials has been suggested for the aerospace or automotive, civil engineering, and other high-performance applications. In membrane applications, polymer/fullerene nanocomposites have been applied due to remarkable morphological, mechanical, barrier, electrical, and other physical properties [195]. In polymer/fullerene nanocomposite membranes, nanofiller dispersal and matrix−nanofiller interactions have been found desirable to develop high-performance nanostructures. Accordingly, the fullerene dispersion has been identified as an important challenge of these membranes. In this regard, modified fullerene derivatives need to be employed. Moreover, precise controls over the pore size, pore structure, microstructure, membrane surface roughness, membrane wettability, etc. (defining the membrane performance parameters) remain as major encounters [196,197]. Furthermore, comprehensive studies are still desired to explore the mechanism of membrane separation processes. Solution-diffusion processes

Challenges, Future, and Summary
There is a mammoth necessity of better-quality approaches to the use of fullerenes and derived nanomaterials in high tech industries [190]. Most prominently, fullerene-derived nanomaterials have been absorbed for membranes or coatings [191], electronics [192], energy devices [193], biomedical areas [194], and other fields. The future implication of fullerene-based nanomaterials has been suggested for the aerospace or automotive, civil engineering, and other high-performance applications. In membrane applications, polymer/fullerene nanocomposites have been applied due to remarkable morphological, mechanical, barrier, electrical, and other physical properties [195]. In polymer/fullerene nanocomposite membranes, nanofiller dispersal and matrix-nanofiller interactions have been found desirable to develop high-performance nanostructures. Accordingly, the fullerene dispersion has been identified as an important challenge of these membranes. In this regard, modified fullerene derivatives need to be employed. Moreover, precise controls over the pore size, pore structure, microstructure, membrane surface roughness, membrane wettability, etc. (defining the membrane performance parameters) remain as major encounters [196,197]. Furthermore, comprehensive studies are still desired to explore the mechanism of membrane separation processes. Solution-diffusion processes leading to water filtration need to be explored experimentally and theoretically, to profoundly identify the separation mechanism. Another important challenge is the discovery of additional all-inclusive categories of polymer/fullerene membranes beyond Nafion/fullerene, polyamide/fullerene, polysulfone/fullerene, and polystyrene/fullerene nanocomposite membranes known so far towards water treatment. The above-mentioned challenges can be overcome by using modified fullerene nanoparticles to attain promising forthcoming membrane nanomaterials. For future membrane utility, the self-assembly of fullerene molecules and network formation with polymeric matrices must be considered [198][199][200].
Consequently, polymer/fullerene nanocomposites capture a special position as separation membranes in the water treatment industry. These membranes have attained increasing research attention due to performance advantages, low operating expenses, high selectivity, and easy scale-up. In fact, the primary function of fullerene has been found as physical/chemical binders within the polymeric chains of nanocomposite membranes for optimizing essential mechanical properties, structural stability, thermal stability, and membrane properties. Certainly, inclusion of fullerene in the matrix creates van der Waals forces and/or covalent interactions with the polymer chains, leading to reinforcement and superior physical features. Moreover, the variations in fullerene loading levels cause dominant effects on the reinforcement and membrane properties. Subsequently, polymer/fullerene nanocomposites have been found as fast emerging separation membranes for clean water resources. Among all available polymer/nanocarbon membranes, polymer/fullerene nanocomposites have been considered as the energy-efficient and green technology for separation of impurities from aqueous solutions due to optimum nanoporous membrane features. Recently, polymer/fullerene nanocomposite membranes have been considered significant for resolving technical and commercial challenges towards separation and purification technologies. The development of distinct polymer/fullerene nanostructured membranes with exclusive properties not only solves the trade-off issue related to water treatment technologies, but also opens new pathways towards real-time applications. The newly fabricated polymer/fullerene membranes have been found superior in terms of selectivity, permeability, and long-term stability. Thus, the research on these novel nanocomposite membranes may continue to develop better cost-effective water treatment systems to decrease the overall capital investment.
In short, this cutting-edge overview grants an analysis on the use of polymer/fullerene C 60 nanocomposite membranes for water remediation. Fullerene and modified fullerene nanofillers have been incorporated in polymers to develop nanocomposite membranes. The enhanced polymer/fullerene nanocomposite properties lead to several prospects to revolutionize the related potential for waste water purification. Plentiful research efforts have been fixated on refining the polymer/fullerene nanocomposite membrane properties such as water permeability, salt rejection, ion separation, overall separation efficiency, antifouling performance, and other membrane topographies. Moreover, fullerene-based nanofillers improve the membrane surface properties, have low cost, and enhance the long-term stability of the membranes. To widen the use of polymer/fullerene in membranes, devotion must be taken to augment polymer-nanocarbon interactions, nanofiller dispersibility, membrane stability, membrane permeability, separation competence, and practicable membrane parameters to solve current glitches in this field.